# Gap modification of atomically thin boron nitride by phonon mediated interactions

- James P Hague
^{1}Email author

**7**:303

https://doi.org/10.1186/1556-276X-7-303

© Hague; licensee Springer. 2012

**Received: **17 January 2012

**Accepted: **23 April 2012

**Published: **14 June 2012

## Abstract

### Abstract

A theory is presented for the modification of bandgaps in atomically thin boron nitride (BN) by attractive interactions mediated through phonons in a polarizable substrate, or in the BN plane. Gap equations are solved, and gap enhancements are found to range up to 70% for dimensionless electron-phonon coupling *λ* =1, indicating that a proportion of the measured BN bandgap may have a phonon origin.

### Keywords

Boron nitride Electron-phonon interactions Semiconductors Two-dimensional materials Graphene## Background

The need for bandgaps in graphene on electronvolt scales has led to a number of proposals, such as the use of bilayer graphene [1], creation of nanoribbons [2], and manipulation through substrates [3, 4]. Recently, it has become possible to manipulate atomically thin layers of boron nitride (BN) and other materials with structure similar to graphene [5]. This may lead to a complimentary method of manipulating bandgaps to make digital transistors.

In low dimensional materials, strong effective electron-electron interactions can be induced via an interaction between electrons confined to a plane and phonons in a polarizable neighboring layer [6]. The theory has shown that similar interactions account for the transport properties of graphene on polarizable substrates [7] and that sandwiching graphene between polarisable superstrates and gap opening substrates can cause gap enhancement [8]. This paper examines similar gap changes in atomically thin BN due to interactions mediated through substrates.

## Methods

*sp*

_{2}hybridization, and electrons with energies close to the chemical potential are in unhybridized

*π*orbitals [9]. A key difference is that the electronic charge is not completely screened by the

*sp*

_{2}hybridization, shifting

*π*orbitals byΔ

_{ n }= + Δ on

*N*sites, and −Δ on

*B*sites. This shift is the dominant cause of a gap of order 2Δ . Tight-binding fits to results from

*ab-initio*simulations of monolayer BN have established the hopping

*t*=2.33 eV [10], with an estimate of Δ =1.96 eV=0.84

*t*. The experiments indicate larger gaps: bulk h-BN has 5.971 eV [11], and monolayer h-BN has a gap of 5.56 eV [12] corresponding to Δ =2.78 eV=1.20

*t*. There is significant variation in phonon energies, $\hslash {\mathrm{\Omega}}_{\mathit{q}}$, in h-BN [13]. Longitudinal acoustic (LA) phonon energies range up to around 140 meV at the

*M*point, and transverse acoustic (TA) modes to around 110 meV at the

*K*point. Optical phonon energies range between 160 and 200 meV. Coupling,

*f*

_{ n }(m), between electrons and phonons in either a polarisable substrate or the BN monolayer, is possible and the corresponding Hamiltonian is as follows:

*σ*on B sites and ${c}_{{\mathit{n}}^{\prime}\sigma}^{\u2020}$ on N sites. Vectors n are to atoms in the monolayer, and m to atoms in the substrate.

*N*

_{ m }and

*n*

_{ n σ }are the number operators for phonons and electrons respectively.

*ξ*

_{ m }is the atomic displacement. The Hamiltonian is also approximately valid for interactions in the plane, and Figure 1 (b) shows the forces on ions from an increase in electron density at a B site. The largest forces are on the near-neighbor sites, so that the effective interaction is mainly site diagonal (electrons on A sites self-interact through phonons on B sites and vice versa). The diagram indicates that the strongest interaction is between electrons and optical phonon modes.

For simplicity, the Holstein electron-phonon interaction was used, ${f}_{\mathit{n}}\left(\mathit{m}\right)\propto {\delta}_{\mathit{n},{\mathit{n}}^{\prime}}$, which qualitatively captures the physics. There may be quantitative changes to the results for longer range Fröhlich interactions and from modulation of the electron-phonon interaction due to incommensurability of the substrate, which was estimated at around ±8*%* of the average value [8].

## Results and discussion

The local approximation used here is a good starting point because the modulated potential Δ is large, and electrons are well localized. Off-diagonal terms do not feature in the lowest order perturbation theory for the Holstein model since the interaction is site diagonal. *Z*_{
n
} is the quasi-particle weight and ${\stackrel{\u0304}{\mathrm{\Delta}}}_{n}$ is the gap function. For bosonic quantities, $\hslash {\omega}_{s}=2\pi {k}_{B}\mathrm{Ts}$ and for fermions, $\hslash {\omega}_{n}=2\pi {k}_{B}T(n+1/2)$. *T* is the temperature and *n* and *s* are integers.

*λ*here is consistent with the mean-field approximation. At half-filling, it is reasonable to assume that

*λ*

_{ A }=

*λ*

_{ B }so thatΔ

^{ A }=Δ

^{ B }and

*Z*

^{ A }=

*Z*

^{ B }. This leads to the gap equations,

where the full gap is ${{\mathrm{\Delta}}^{\prime}}_{n}={\stackrel{\u0304}{\mathrm{\Delta}}}_{n}+\mathrm{\Delta}$. The density of states for a tight binding hexagonal lattice in the absence of a gap, *D* (*ε* ), has the form given in reference [14]. The equations may be solved self-consistently by performing a truncated sum on Matsubara frequencies.

*%*for $\lambda =1,\phantom{\rule{2.77695pt}{0ex}}{k}_{B}T=\hslash \mathrm{\Omega}=0.01t$). The local gap enhancement factorsΔ

^{ ′ }/Δ, are shown in Figure 2 (a) for various

*λ*, showing a modest increase of around 70% for

*λ*=1. The enhancement factor increases slightly with decreasing Δ but is essentially unchanged by modifications to phonon frequency and temperature for the parameter values used here. The temperature dependence of the gap was also calculated in Figure 2 (b). For very large temperatures, where

*k*

_{B}

*T*approaches Δ , there is a drop in the gap size. Below approximately 8,000 K (0.3

*t*), this levels off, and the gap becomes relatively constant.

## Conclusions

A theory for the modification of BN band-gaps by interaction with phonons was presented here. It is of interest to make a comparison between the bandgaps of bulk h-BN, nanotubes, monolayer h-BN, and the theory presented here. Measured bandgaps of bulk h-BN are of between 5.8 eV [15] and 5.971 eV [11], indicating that interaction between layers increases the bandgap, consistent with the theory here. The bulk gap is also higher than that for nanotubes (5 eV) [16]. On the other hand, Song et al. [12] claim that the gap is reduced as BN thickness increases. The above discussion is presented with a warning that the theory requires that hopping between the substrate and the BN monolayer is small. Interlayer hopping will affect the bandwidth and bandgap, and the direct Coulomb interaction with strongly ionic substrates could also affect the band structure if the charge density at the surface of the substrate varies dramatically.

It is also of interest to estimate the magnitude of the bandgap modification due to electron-phonon interaction in isolated monolayers of BN. *Ab initio* calculations have attempted to quantify the magnitude of the interaction between electrons and acoustic phonons for small momentum excitations [17]. Extrapolating the interaction and taking a mean-field average (assuming mean momentum magnitude of 4*π* /9*a* ), the electron-phonon coupling can be estimated as $\lambda ={(4\pi /9)}^{2}{E}_{1}^{2}/2{a}^{2}t\stackrel{\u0304}{M}{\mathrm{\Omega}}^{2}$, taking *E*_{1}=3.66 eV from reference [17], $\stackrel{\u0304}{M}\approx 12.5$ amu, a=2.5Å. The mean energy of longitudinal acoustic phonons lies in the range of 50 to 75 meV, giving a range of *λ* =0.05 to 0.12, so the contribution of phonons to the bandgap is estimated as 3% to 7%. I would expect BN to have stronger interaction with optical phonons, since the pattern of distortions around an electronic defect is consistent with optical modes (see Figure 1).

The BN gap is too wide for digital applications. Recently, it has become possible to manufacture silicene, an atomically thick layer of silicon with similar properties to graphene [18], so it may be possible to make GaAs or AlP analogues to BN. Smaller gaps could be available from those materials, which might be used to create tunable bandgaps for atomically thick transistors.

## Author’s information

JPH is a lecturer from the Faculty of Science, Department of Physical Sciences, The Open University, Walton Hall, Milton Keynes, UK.

## Declarations

### Acknowledgements

The author acknowledges EPSRC grant EP/H015655/1 for funding and useful discussions with A Ilie and A Davenport.

## Authors’ Affiliations

## References

- McCann E, Fal’ko VI: Landau-level degeneracy and quantum hall effect in a graphite bilayer.
*Phys Rev Lett*2006, 96: 086805.View ArticleGoogle Scholar - Brey L, Fertig HA: Electronic states of graphene nanoribbons studied with the Dirac equation.
*Phys Rev B*2006, 73: 235411.View ArticleGoogle Scholar - Zhou SY, Gweon GH, Fedorov AV, First PN, Heer WAD, Lee DH, Guinea F, Neto AHC, Lanzara A: Substrate-induced bandgap opening in epitaxial graphene.
*Nature Materials*2007, 6: 770. 10.1038/nmat2003View ArticleGoogle Scholar - Enderlein C, Kim YS, Bostwick A, Rotenberg E, Horn K: The formation of an energy gap in graphene on ruthenium by controlling the interface.
*New J Phys*2010, 12: 033014. 10.1088/1367-2630/12/3/033014View ArticleGoogle Scholar - Novoselov KS, Jiang D, Schedin F, Booth TJ, Khotkevich VV, Morozov SV, Geim AK: Two-dimensional atomic crystals.
*Proc Natl Acad Sci USA*2005, 102: 10451. 10.1073/pnas.0502848102View ArticleGoogle Scholar - Alexandrov AS, Kornilovitch PE: The Fröhlich-Coulomb model of high-temperature superconductivity and charge segregation in the cuprates.
*J Phys: Condens Matter*2002, 14: 5337. 10.1088/0953-8984/14/21/308Google Scholar - Fratini S, Guinea F: Substrate-limited electron dynamics in graphene.
*Phys Rev B*2008, 77: 195415.View ArticleGoogle Scholar - Hague J: Tunable graphene band gaps from superstrate-mediated interactions.
*Phys Rev B*2011, 84: 155438.View ArticleGoogle Scholar - Alem N, Erni R, Kisielowski C, Rossell M, Gannett W, Zettl A: Band-gap engineering and ballistic transport in edge-corrugated graphene nanoribbons.
*Phys Rev B*2009, 80: 155425.View ArticleGoogle Scholar - Ribeiro RM, Peres NMR: Stability of boron nitride bilayers: ground-state energies, interlayer distances, and tight-binding description.
*Phys Rev B*2011, 83: 235312.View ArticleGoogle Scholar - Watanabe K, Taniguchi T, Kanda H: Direct-bandgap properties and evidence for ultraviolet lasing of hexagonal boron nitride single crystal.
*Nat Mater*2004, 3: 404. 10.1038/nmat1134View ArticleGoogle Scholar - Song L, Ci L, Lu H, Sorokin P, Jin C, Ni J, Kvashnin A, Kvashnin D, Lou J, Yakobson B, Ajayan P: Large scale growth and characterization of atomic hexagonal boron nitride layers.
*Nano Lett*2010, 10: 3209. 10.1021/nl1022139View ArticleGoogle Scholar - Serrano J, Bosak A, Arenal R, Krisch M, Watanabe K, Taniguchi T, Kanda H, Rubio A, Wirtz L: Vibrational properties of hexagonal boron nitride: inelastic X-Ray scattering and ab initio calculations.
*Phys Rev Lett*2007, 98: 095503.View ArticleGoogle Scholar - Neto AHC, Guinea F, Peres NMR, Novoselov KS, Geim AK: The electronic properties of graphene.
*Rev Mod Phys*2009, 81: 109. 10.1103/RevModPhys.81.109View ArticleGoogle Scholar - Zunger A, Katzir A, Halperin A: Optical properties of hexagonal boron nitride.
*Phys Rev B*1976, 13: 5560. 10.1103/PhysRevB.13.5560View ArticleGoogle Scholar - Terauchi M, Tanaka M, Matsumoto T, Saito Y: Electron energy-loss spectroscopy study of the electronic structure of boron nitride nanotubes.
*J Electron Microscopy*1998, 47: 319. 10.1093/oxfordjournals.jmicro.a023598View ArticleGoogle Scholar - Bruzzone S, Fiori G: Ab-initio simulations of deformation potentials and electron mobility in chemically modified graphene and two-dimensional hexagonal boron-nitride.
*Appl Phys Lett*2011, 99: 222108. 10.1063/1.3665183View ArticleGoogle Scholar - Padova PD, Quaresima C, Ottaviani C, Sheverdyaeva P, Moras P, Carbone C, Topwal D, Olivieri B, Kara A, Oughaddou H, Aufray B, Lay GL: Evidence of graphene-like electronic signature in silicene nanoribbons.
*Appl Phys Lett*2010, 96: 261905. 10.1063/1.3459143View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License(http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.